A Chapter in Scaffolding in Tissue Engineering
PuraMatrix: Self-assembling Peptide Nanofiber Scaffolds
Shuguang Zhang*, Rutledge Ellis-Behnke, Xiaojun Zhao, and Lisa Spir io
Center for Biomedical Engineer ing, NE47-379,
*Center for Bits & Atoms Depar tment of Brain and Cognitive Science
Massachusetts Institute of Technology
77 Massachusetts Avenue
Cambr idge, MA 02139-4307 3-DMatr ix, Inc., Cambr idge, MA, www.puramatr ix.com
Tel.: 617-258-7514, FAX: 617-258-0204
Table of Content 1. INTRODUCTION
1.1. Animal-derived ECM and synthetic scaffolds 1.2. PuraMatrix Peptide Nanofiber Scaffolds Nanofiber-scale synthetic ECM Defined 3-D microenvironments for cell biology 1.3 3-D Cell Culture Versus 2-D 1.4. Nanoscale Fibers Versus Microscale 1.5. Ideal synthetic biological scaffolds
2. SELF-ASSEMBLING PEPTIDES 2.1. Discovery and Development of Self-assembling Peptides.
Simple repeating units of amino acids assemble into nanofiber scaffolds
Amenable to design incorporating bioactive elements
2.2. Structural Properties of Self-assembling Peptides
3. PEPTIDE NANOFIBER SCAFFOLDS 3.1. EAK16-II 3.2. RADA16 3.3. KFE8 and KLD12
4. PURAMATRIX IN VITRO CELL CULTURE EXAMPLES. 4.1. Hepatocytes 4.2. Adult Liver Progenitor Cells 4.3. Chondrocytes Form Molded Cartilage in Cell Culture 4.4. Extensive Neurite Outgrowth and Active Synapse Formation on PuraMatrix
4.5. Organotypic Hippocampal Tissue Culture in PuraMatrix 4.6. Murine Embryonic Stem Cells 4.7. Osteoblasts
5. STANDARD IN VITRO TOXICOLOGY AND BIOCOMPATIBILITY STUDIES 5.1. Cytotoxicity 5.2. Hemolysis 5.3. Coagulation Prothrombin Time
6. IN VIVO BIOCOMPATIBILITY AND TOXICOLOGY STUDIES 6.1. ADME and Biodegradability 6.2. Rabbit Muscle Implant (2 weeks) 6.3. Peptide Nanofiber Scaffold for Brain Lesion Repair in Hamsters. 6.4. Intracutaneous Reactivity 6.5. Rabbit Pyrogen
7. FUTURE PERSPECTIVE 7.1. Forward-Compatible with Bioproduction and Clinical Applications. 7.2. Synthetic Origin, Clinical-Grade Quality, Clinical Delivery. 7.3. Tailor-made PuraMatrix
The fields of tissue engineering and reparative and regenerative medicine require two key complementary components: 1) a suitable biological scaffold that creates a microenvironment niche for a given cell type, and 2) that the given cell type can rapidly integrate and coalesce into the needed tissue.
The three-dimensional assembly of cells in a biological microenvironment is designed to recapitulate normal tissue function (1). Often this involves the use of biomaterials. The task of the biomedical engineering is to design and to select optimal biomaterials with the properties most closely matched to those needed for a particular application (2-6).
Stem cells and phenotypically plastic cells hold high hopes for tissue engineering, reparative and regenerative medicine. In most cases, these cells must be paired with microenvironments, which instruct proper expansion and/or differentiation, through mimicry of the native in vivo microenvironments and basement membranes and with a critical constituent being the extracellular matrix (ECM) (7-9). This fibrous protein scaffold not only provides the appropriate three-dimensional architecture, but also promotes signaling pathways influencing critical cell functions such as proliferation, differentiation, and migration (10-11). Moreover, the fields of tissue engineering, stem cell biology, and cancer biology are realizing that the ECM and a fine-tuned three-dimensional microenvironment are critical for the proper understanding and manufacturing of successful clinically-relevant therapies.
However, most cell biology research has used two-dimensional constructs to study single cell populations treated selectively with soluble factors in a homogeneous environment (12). This greatly simplifies the research models, but also mitigates the powerful effects of ECM and 3-D culture conditions on the cells of interest. Recreating 3-D conditions and structures in vitro, rather than growing cells in 2-D Petri dishes and flasks, have yielded tools for more accurate biological analyses (13, 14).
1.1. Animal-derived ECM and synthetic scaffolds
In the past two decades have witnessed the quest for synthetic biocompatible polymers, hydrogels, and or animal-derived materials (2-6). Until recently, 3-D cell culture has required either synthetic scaffolds, which fail to approximate the physical nanoscale size and chemical attributes of native ECM, or animal-derived materials, which may confound cell culture with undefined or inconsistent variables. Biomaterials such as PLLA and PGA biopolymers, calcium phosphate mesh, PEG gels, methylcellulose, alginates and agarose have seen limited success, partly due to either their large microfiber size relative to cells, acidic breakdown products, charge density, lower nutrient diffusion rates, or inability to allow the creation of functional microenvironments by the cells. Animal derived biomateials including bovine collagen and gelatin, fibronectin, intestinal submucosa, cadaver tissue, and Matrigel may help to create the right microenvironments, but complicate research and therapies with their potential risk of other unknown material contaminations, thus rise issues about cell signaling, protein content, and reproducibility.
We have described a family of synthetic self-assembling peptide scaffolds (SAPS), which we now call PuraMatrix because of its synthetic nature and extreme purity of a single peptide component. PuraMatrix not only can be used as a coating or to encapsulate cells similar to the ECM, but can also be tailor-made for particular cells, tissues and therapies.
1.2. PuraMatr ix Peptide Nanofiber Scaffolds
Over the past 10 years, a new class of biologically-inspired peptide biomaterials has been discovered and developed in the context of cell culture, stem cell biology and tissue engineering. These self-assembling peptide scaffolds have been used successfully as a synthetic in vitro and in vivo ECM, proving themselves as a critical component to successful 3-D cell growth.
Nanofiber-scale synthetic ECM
PuraMatrix is a 16 amino acid synthetic peptide that is resuspended in water to generate a range of solution concentrations. Upon the introduction of millimolar amounts of monovalent cations, either through the addition of salt solution, cell culture media or injection of the material in vivo, PuraMatrix undergoes self-assembly into nanofibers, ~10 nm in diameter, on a scale similar to the in vivo extracellular matrix (ECM). The physical size relative to cells and proteins, the amphiphilic peptides charge density, and water-structuring abilities mimic the in vivo ECM. These well-ordered nanofibers create 3-dimensional porous scaffolds that are very difficult or impossible to synthetically produce by other manufacturing techniques. The nanofiber density and average pore size, ~5-200 nm, correlates with the concentration of peptide solution that is used to produce the material, which can be varied from 0.1 to 3% in water (1-30mg/ml w/v) depending on the application.
Defined 3-D microenvironments for cell biology
PuraMatrix mimics several important aspects of the in vivo environment a synthetic ECM enabling defined cell culture conditions while allowing cells to proliferate and differentiate within a 3-D context, easily migrate within that microenvironment, and create their own microenvironments quickly including production of their own ECM.
1.3. 3-D Cell Culture Versus 2-D
The advancement of biological study often requires the development of new materials, methods and tools. The introduction of the Petri dish over 100 years ago provided an indispensable tool for culturing cells in vitro, thus permitting the detailed dissection of seemingly intractable biology and physiology systems into manageable units and well-defined studies. This simple dish has had profound impact on our understanding of complex biology, especially cell biology and neurobiology.
However, the Petri dish culture system, including multi-well plates, glass cover slips, etc, is less than ideal for several reasons: 1) It is a 2-dimensional (2-D) system which is in sharp contrast to the 3-D environment of natural tissues both animal and plant. 2) The Petri dish surface without coating is rigid and inert, again in sharp contrast to the in vivo
environment where cells intimately interact with the extracellular matrix and with each other. 3) The tissue cell monolayers on coated 2-D surface, such as poly-L-lysine, collagen gels, fibronectin, and laminin as well as other synthetic materials containing segments of adhesion motifs, have only part of the cell surface attached to the materials and interact neighboring cells. The remaining parts are often directly exposed to the culture media, unlike the tissue environment where every cell intimately interact with its neighbors and the ECM. 4) The transport phenomena of 2-D and 3-D are drastically different. In 2-D culture systems, cytokines, chemokines and growth factors quickly diffuse in the media across the culture dish. This is again in sharp contrast to the in vivo environment where chemical and biological gradients play a vital role in signal transduction, chemotaxis, cell-cell communications and development. Cells respond to local concentrations of a variety of molecules, which in traditional cell culture, are distributed homogenously. Yet, most cells, by virtu